Upload
phamnhu
View
222
Download
0
Embed Size (px)
Citation preview
440 ACI Structural Journal/July-August 2008
ACI Structural Journal, V. 105, No. 4, July-August 2008.MS No. S-2006-478 received December 11, 2006, and reviewed under Institute
publication policies. Copyright © 2008, American Concrete Institute. All rights reserved,including the making of copies unless permission is obtained from the copyright proprietors.Pertinent discussion including author’s closure, if any, will be published in the May-June 2009 ACI Structural Journal if the discussion is received by January 1, 2009.
ACI STRUCTURAL JOURNAL TECHNICAL PAPER
A mechanical explanation of the phenomenon of punching shear inslabs without transverse reinforcement is presented on the basis ofthe opening of a critical shear crack. It leads to the formulation ofa new failure criterion for punching shear based on the rotation ofa slab. This criterion correctly describes punching shear failuresobserved in experimental testing, even in slabs with low reinforcementratios. Its application requires the knowledge of the load-rotationrelationship of the slab, for which a simple mechanical model isproposed. The resulting approach is shown to give better resultsthan current design codes, with a very low coefficient of variation(COV). Parametric studies demonstrate that it correctly predictsseveral aspects of punching shear previously observed in testing assize effect (decreasing nominal shear strength with increasing sizeof the member). Accounting for the proposed failure criterion andload-rotation relationship of the slab, the punching shear strengthof a flat slab is shown to depend on the span of the slab, ratherthan on its thickness as often proposed.
Keywords: critical shear crack; interior slab-column connection; punchingshear; two-way shear.
INTRODUCTIONReinforced concrete slabs on columns were initially
developed in the U.S. and Europe at the beginning of the20th century.1,2 Their designs typically included largemushroom-shaped column capitals to facilitate the localintroduction of forces from the slab to the column. In the1950s, flat slabs without capitals started to become prevalent.Because of their simplicity, both for construction and for use(simple formwork and reinforcement, flat soffit allowing aneasy placement of equipment, and installation underneaththe slab), they have become very common for mediumheight residential and office buildings as well as for parkinggarages. The design of flat slabs is mostly governed byserviceability conditions on the one side (with relativelylarge deflections in service) and by the ultimate limit state ofpunching shear (also called two-way shear) on the other side.These two criteria typically lead to the selection of theappropriate slab thickness.
Punching shear has been the object of an intense experimentaleffort since the 1950s. In most cases, the phenomenon isinvestigated by considering an isolated slab element. Thiselement typically represents the surface of the slabsurrounding a column and is delimited by the line ofcontraflexure for radial moments, which are zero at adistance rs ≈ 0.22L (according to a linear-elastic estimate),where L is the axis-to-axis spacing of the columns. In recentyears, several state-of-the-art reports and synthesis papershave been published on this topic.3-5
Most design codes base their verifications on a criticalsection, with the punching shear strength of slabs withoutshear reinforcement defined as a function of the concretecompressive strength and often of the reinforcement ratio.
Some codes also account for size effect, membrane effect, orthe ratio of column size to the depth of the slab. Equation (1)shows the ACI 318-056 expression for square or circularcolumns of moderate dimensions relative to the thickness ofthe slab
(1)
where d is the average flexural depth of the slab, b0 is theperimeter of the critical section located d/2 from the face of thecolumn, and fc′ is the specified concrete compressive strength.
The current version of Eurocode 27 also includes a formu-lation for estimating the punching shear strength of slabs
(2)
where b0 is the control perimeter located 2d from the face ofthe column, ρl accounts for the bending reinforcement ratio(with a maximum value of 0.02) and ξ is a factor accountingfor size effect defined by the following expression
(3)
In the early 1960s, Kinnunen and Nylander8 tested a seriesof slabs in punching, varying amongst other parameters theamount of flexural reinforcement in the slab (refer to Fig. 1).The following observations can be made from the load-rotationrelationships of the tests:• For low reinforcement ratios (test with ρ = 0.5%), the
observed behavior is ductile, with yielding of the entireflexural reinforcement, as illustrated by the horizontalasymptote of the load-rotation curve. In this case, thestrength of the slab is limited by its flexural capacityand punching occurs only after large plastic deformations.The punching failure at the end of the plastic plateauremains brittle and leads to a sudden drop in strength;
VR13---b0d fc′ (SI units: MPa, mm)=
VR 4b0d fc′ (U.S. customary units: psi, in.)=
VR 0.18b0dξ 100ρl fc ′( )
13---
(SI units: MPa, mm)=
VR 5.0b0dξ 100ρl fc ′( )
13---
(U.S. customary units: psi, in.)=
ξ 1 200 mmd
--------------------+ 1 7.87 in.d
------------------ 2.0≤+= =
Title no. 105-S42
Punching Shear Strength of Reinforced Concrete Slabs without Transverse Reinforcementby Aurelio Muttoni
441ACI Structural Journal/July-August 2008
• For intermediate reinforcement ratios (tests with ρ =1.0%/0.5% and 1.0%), some yielding of the reinforcementis present in the immediate vicinity of the column, butpunching occurs before yielding of the entire slabreinforcement. In this case, the strength of the slab islower than its flexural capacity;
• For large reinforcement ratios (test with ρ = 2.1%/1.0%),punching occurs before any yielding of the reinforcementtakes place, in a very brittle manner. In this case, thestrength of the slab is significantly lower than itsflexural capacity;
• Increasing the reinforcement ratio increases the punchingcapacity, but strongly decreases the deformation capacityof the slab; and
• The ACI design equation is also plotted in the figure. Itpredicts a constant strength independent from thereinforcement ratio. As observed by Alexander andHawkins,9 Eq. (1) is basically a design equation; as such, itdoes not account for the effect of the flexural reinforcement.
On the basis of their test results, Kinnunen and Nylander8
developed a rational theory for the estimation of thepunching shear strength in the early 1960s based on theassumption that the punching strength is reached for a givencritical rotation ψ. This rotation was calculated bysimplifying the kinematics of the slab and assuming abilinear moment-curvature relationship. Thus far, this proposalremains one of the best models for the phenomenon ofpunching. Recently, some improvements were proposed byHallgren10 and Broms11 to account for size effects and high-strength concrete. While very elegant and leading to goodresults, this model was never directly included in codes of prac-tice because its application is too complex. It served as a basis,however, for the Swedish and Swiss design codes of the 1960s.
RESEARCH SIGNIFICANCERational models and design formulas for punching shear,
or two-way shear, are based on the results of experimentaltests performed mostly on thin slabs (d = 0.1 to 0.2 m [4 to8 in.]). Design codes, however, are generally also applicableto thick slabs and footings (0.4 m [16 in.] and more). The fewavailable tests performed on thick slabs exhibit a notable sizeeffect. As a consequence, there is a need for a rational modelcorrectly describing punching shear and accounting for sizeeffect (defined as decreasing nominal shear strength withincreasing size of the member).
In this paper, a new failure criterion for punching shear basedon the critical shear crack theory is presented. This criteriondescribes the relationship between the punching shear strengthof a slab and its rotation at failure, it is consistent with the worksof Kinnunen and Nylander8 and it accounts for size effect. Theresulting equations are presented in a code-friendly formulation.
FAILURE CRITERION BASED ON CRITICAL SHEAR CRACK THEORY
Critical shear crack theoryAs shown in Fig. 1, the punching shear strength decreases
with increasing rotation of the slab. This has been explained
by Muttoni and Schwartz12 as follows: the shear strength isreduced by the presence of a critical shear crack that propagatesthrough the slab into the inclined compression strut carryingthe shear force to the column (Fig. 2(b)). Some evidencessupporting the role of the shear critical crack in the punchingshear strength are detailed in the following:
1. It has been shown experimentally8,13 that the radialcompressive strain in the soffit of the slab near the column,after reaching a maximum for a certain load level, begins todecrease (Fig. 2(d)). Shortly before punching, tensile strainsmay be observed. This phenomenon can be explained by thedevelopment of an elbow-shaped strut with a horizontaltensile member along the soffit due to the development of thecritical shear crack12 (Fig. 2(c)). A similar phenomenon hasbeen observed in beams without shear reinforcement12; and
2. Experimental results by Bollinger14 also confirm therole of the critical shear crack in the punching strength ofslabs. The tested slab shown in Fig. 3(b) was reinforced byconcentric rings placed at the boundary of the slab elementonly. With this particular reinforcement layout, only radialcracks developed and the formation of circular cracks in thecritical region was avoided. Thus, the punching shearstrength of this test was significantly larger than that of asimilar slab with an additional ring in the critical region(Fig. 3(c)). For this test, the presence of an additional ring inthe vicinity of the critical region initiated the development ofa crack in that region, with a subsequent reduction of thepunching shear strength of approximately 43%.
Punching shear strength as function ofslab rotation
The opening of the critical shear crack reduces the strengthof the inclined concrete compression strut carrying shear andeventually leads to the punching shear failure. According toMuttoni and Schwartz,12 the width of the critical crack canbe assumed to be proportional to the product ψd (Fig. 4),leading to a semi-empirical failure criterion formulated in 1991 as
ACI member Aurelio Muttoni is a Professor and Head of the Structural ConcreteLaboratory at the Ecole Polytechnique Fédérale de Lausanne (EPFL), Lausanne,Switzerland. He received his diploma and PhD in civil engineering from the SwissFederal Institute of Technology, Zurich, Switzerland, in 1982 and 1989, respectively.His research interests include the theoretical basis of the design of reinforced concretestructures, shear and punching shear, fiber-reinforced high-strength concrete, soil-structure interaction, and the conceptual design of bridges.
Fig. 1—Plots of load-rotation curves for tests by Kinnunenand Nylander8 (geometric and mechanical parameters oftests defined in Fig. 8).
442 ACI Structural Journal/July-August 2008
(4)
The amount of shear that can be transferred across the criticalshear crack depends on the roughness of the crack, which inits turn is a function of the maximum aggregate size.According to Walraven15 and Vecchio and Collins,16 theroughness of the critical crack and its capacity to carry theshear forces can be accounted for by dividing the nominalcrack width ψd by the quantity (dg0 + dg), where dg is themaximum aggregate size, and dg0 is a reference size equal to16 mm (0.63 in.). It should be noted that the value of dg hasto be set to zero for lightweight aggregate concrete toaccount for cracks developing through aggregates. On thatbasis, in 2003 Muttoni17 proposed an improved formulationfor the failure criterion
(5)
Figure 5 compares the results obtained with Eq. (5) to theresults of 99 punching tests from the literature, for whichTable 1 provides additional information. In this figure, theslab rotation was either obtained from direct measurementsor calculated by the author from the measured deflection,assuming a conical deformation of the slab outside the
VE
b0d fc3
----------------- 1
1 ψd4mm------------⎝ ⎠⎛ ⎞ 2
+
------------------------------= (SI units; N, mm)
VR
b0d fc3
----------------- 28
1 ψd0.16 in. --------------------⎝ ⎠⎛ ⎞ 2
+
-------------------------------------= U.S. customary units; psi, in.)
VR
b0d fc
----------------- 3 4⁄
1 15 ψddg0 dg+-------------------+
----------------------------------- (SI units: N, mm)=
VR
b0d fc
----------------- 9
1 15 ψddg0 dg+-------------------+
----------------------------------- (U.S. customary units: psi, in.)=
Fig. 3—Tests by Bollinger14 with ring reinforcements, effectof additional reinforcement in vicinity of critical shearcrack on load-carrying capacity: (a) test results; and (b)and (c) reinforcement layout of Specimens 11 and 12.
Fig. 4—Correlation between opening of critical shearcrack, thickness of slab, and rotation ψ.
Fig. 2—Test PG-3 by Guandalini and Muttoni13 (geometric and mechanical parameters oftest defined in Fig. 9): (a) cracking pattern of slab after failure; (b) theoretical strutdeveloping across the critical shear crack; (c) elbow-shaped strut; and (d) plots ofmeasured radial strains in soffit of slab as function of applied load.
ACI Structural Journal/July-August 2008 443
column region. In cases where different reinforcement ratioswere placed along orthogonal directions, the maximum rotationof the slab was considered. The rotation ψ is multiplied bythe factor d/(dg0 + dg) to cancel the effects of slab thicknessand aggregate size. Tests in which punching shear failureoccurred after reaching the flexural strength Vflex are alsoconsidered (shown as empty squares in the figure).
The expression provided in ACI 318-056 is also plotted inFig. 5. It can be noted that for small values of ψd/(dg0 + dg),the code gives rather conservative results. This is also the area ofthe plot in which the majority of the tests are located. For largevalues of ψd/(dg0 + dg), however, the ACI equation predictssignificantly larger punching shear strengths than effectivelyobserved in tests. This fact can be traced back to two causes:
1. When the ACI formula was originally proposed in theearly 1960s,9,19 only tests with relatively small effectivedepths were available and the influence of size effect wasthus not apparent; and
2. Tests in which punching failure occurred after reachingthe flexural strength but with limited rotation capacity areconsidered in the comparison (empty squares).
LOAD-ROTATION RELATIONSHIPComparing Fig. 1 and 5, it is clear that the punching failure
occurs at the intersection of the load-rotation curve of theslab with the failure criterion. To enable a calculation of thepunching shear strength according to Eq. (5), the relationshipbetween the rotation ψ and the applied load V needs to beknown. In the most general case, the load-rotation relationshipcan be obtained by a nonlinear numerical simulation of theflexural behavior of the slab, using, for example, a nonlinearfinite element code. In axisymmetric cases, a numericalintegration of the moment-curvature relationship can beperformed directly.26 This allows to account for bendingmoment redistributions in flat slabs and to account for theincrease on punching shear strength due to in-plane confinementgiven by the flat slab in the portions of the slab near columns.26
The axisymmetric case of an isolated slab element can alsobe treated analytically after some simplifications. As alreadydescribed, the tangential cracks and the radial curvature are
concentrated in the vicinity of the column. Outside the criticalshear crack, located at a radius r0 (assumed to be at a distanced from the face of the column), the radial moment, and thusthe radial curvature, decreases rapidly as shown in Fig. 6(d)and (e). Consequently, it can be assumed that the correspondingslab portion deforms following a conical shape with aconstant slab rotation ψ (Fig. 6(a)).
In the region inside the radius r0, the radial moment isconsidered constant because the equilibrium of forces isperformed along cross sections defined by the shape of theinclined cracks (Fig. 6(b) and (c)), where the force in thereinforcement remains constant (due to the fact that the shearforce is introduced in the column by an inclined strut developingfrom outside the shear critical crack (Fig. 2(b) and (c)).
The full development of the expressions for the load-rotationrelationship of the slab is given in Appendix 1.* Considering aquadrilinear moment-curvature relationship for the reinforcedconcrete section (Fig. 7), the following expression results
(6)
where mr is the radial moment per unit length acting in the slabportion at r = r0 and the operator ⟨x⟩ is x for x ≥ 0 and 0 for x < 0.
A simpler moment-curvature relationship can be adoptedby neglecting the tensile strength of concrete fct and theeffect of tension stiffening, leading to a bilinear relationshipsimilar to that of Kinnunen and Nylander,8 shown as a dottedline in Fig. 7. The analytical expression describing the load-rotation relationship is thus
V 2πrq rc–-------------- mrr0– mR ry r0–⟨ ⟩ EI1ψ r1( ) ry( )ln–ln⟨ ⟩+ + +
EI1χTS r1 ry–⟨ ⟩ mcr rcr r1–⟨ ⟩ EI0ψ rs( ) rcr( )ln–ln⟨ ⟩+ +⎝ ⎠⎜ ⎟⎛ ⎞
=
Fig. 5—Failure criterion: punching shear strength as functionof width of critical shear crack compared with 99 experimentalresults and ACI 318-056 design equation, refer to details oftest series in Table 1.
Table 1—Test series considered in present study and comparison with proposed failure criterion
Reference (year) d, mm (in.) No.
Failure criterion Vtest/Vth
Average COV
Tests with same bending reinforcement ratio along orthogonal directions
Elstner and Hognestad18 (1956) 115 (4.52) 22 0.98 0.14
Kinnunen and Nylander8 (1960) 122 (4.80) 12 1.05 0.11
Moe19 (1961) 114 (4.48) 9 1.13 0.16
Schäfers20 (1984)113 to 170
(4.45 to 6.69) 4 1.03 0.20
Tolf21 (1988)98 to 200
(3.86 to 7.87) 8 1.06 0.15
Hassanzadeh22 (1996) 200 (7.87) 3 0.99 0.17
Hallgren10 (1996) 199 (7.83) 7 0.98 0.25
Ramdane23 (1996) 98 (3.86) 12 1.10 0.16
Guandalini and Muttoni13 (2004)96 to 464
(3.78 to 18.2) 10 1.11 0.22
Σ 87 1.05 0.16
Tests with different bending reinforcement ratio along orthogonal directions
Nylander and Sundquist24 (1972)95 to 202
(3.74 to 7.95) 11 1.04 0.09
Kinnunen et al.25 (1980) 673 (26.5) 1 0.85 —
Σ 12 1.03 0.10
Note: COV = coefficient of variation.
*The Appendixes are available at www.concrete.org in PDF format as an addendumto the published paper. It is also available in hard copy from ACI headquarters for afee equal to the cost of reproduction plus handling at the time of the request.
444 ACI Structural Journal/July-August 2008
(7a)
(7b)
The flexural strength of the slab specimen is reached whenthe radius of the yielded zone (ry) equals the radius of the slabrs. In this case (ry = rs = r1 = rcr, and –mr = mR), Eq. (6) yields
(7c)
V 2πrq rc–---------------EI1ψ 1
rs
r0
----ln+⎝ ⎠⎛ ⎞ for ry r0 (elastic regime)≤=
V 2πrq rc–--------------EI1ψ 1
rs
ry
----ln+⎝ ⎠⎛ ⎞ for r0 ry rs (elasto-plastic regime)≤ ≤=
Vflex 2πmRrs
rq rc–--------------- (plastic regime)=
Figure 8 shows a comparison of the proposed solutionswith the previously described tests by Kinnunen andNylander8 (Fig. 1). The solid curves represent the solution
Fig. 6—Assumed behavior for axisymmetric slab: (a)geometrical parameters and rotation of slab; (b) forces inconcrete and in reinforcement acting on slab sector; (c)internal forces acting on slab sector; (d) distribution ofradial curvature; (e) distribution of radial moment; (f)distribution of tangential curvature; and (g) distribution oftangential moments for quadrilinear moment-curvaturerelationship (shaded area) and for bilinear moment-curvaturerelationship (dashed line).
Fig. 7—Moment-curvature relationships: bilinear andquadrilinear laws.
Fig. 8—Tests by Kinnunen and Nylander8: (a) comparisonof load-rotation curves for tests and for proposed analyticalexpressions (Eq. (6) and (7)); (b) dimensions of specimens;and (c) mechanical parameters.
ACI Structural Journal/July-August 2008 445
with a quadrilinear moment-curvature relationship of Eq. (6),whereas the dotted curves show the simplified solution witha bilinear moment-curvature relationship of Eq. (7). For thethin slabs of Fig. 8, both solutions predict the punching load forall reinforcement ratios very well. It may be noted, however,that the distance between the two solutions is larger forsmaller reinforcement ratios at lower load levels. In thesecases, Eq. (6) (which uses a quadrilinear moment-curvaturerelationship) predicts the full load-rotation relationship withgood accuracy. Equation (7), with a simplified bilinearmoment-curvature relationship, gives adequate but lessaccurate results, especially for low load levels, in which thetensile strength of concrete and tension stiffening effects aremore pronounced. Both approaches correctly describe theactual rotation capacity of the slab at failure. The punchingshear strength can be obtained directly by substituting Eq. (6)or (7) into Eq. (5) and solving the resulting equation.
Influence of thickness of slabFigure 9 shows the load-rotation curves for two tests by
Guandalini and Muttoni.13 These two tests are very similar,with the same reinforcement ratio (ρ = 0.33%) and the samemaximum aggregate size (dg = 16 mm [0.63 in.]). Whatdistinguishes them is the dimensions of the slabs: Slab PG10is 3.0 x 3.0 x 0.25 m (118 x 118 x 9.8 in.), whereas Slab PG3is twice as large 6.0 x 6.0 x 0.5 m (236 x 236 x 19.7 in.). Tofacilitate the comparison of these two tests, the abscissa,contrary to the previous figures, shows the actual slab rotation,not the value corrected for aggregate size and size effect. Inthis representation, the load-rotation relationship of bothslabs is nearly identical, as they are geometrically identical,but scaled 2:1. The failure criteria, however, are differentdue to their different thicknesses. This is why two dottedlines are shown, giving the failure criterion of Eq. (5) foreach slab thickness, the upper applying to the thinner and thelower to the thicker slab. In the latter case, with a lowreinforcement ratio, the difference between the two load-rotation relationships, with and without tension stiffening,becomes apparent, whereas the more accurate expression ofEq. (6) quite closely predicts the entirety of the loadingcurve, the simpler solution of Eq. (7) clearly underestimates thestiffness of the slab in its initial loading stages, thus leadingto an underestimation of the punching shear strength.Whereas both equations give conservative estimates of the actualfailure load, only Eq. (6) correctly describes all stages of theactual behavior of the thick slab with a small reinforcementratio. Because both slabs are geometrically similar andbecause of size effect, the thicker slab has a lower rotationcapacity and fails in a rather brittle manner, in spite of its lowreinforcement ratio, whereas the thinner slab exhibits a moreductile behavior.
Figure 10 further illustrates this phenomenon by showingthe load-rotation curves according to Eq. (6) for variousreinforcement ratios, along with the failure criteria forvarious slab thicknesses. The constant value predicted by theACI 318-056 design equation is also shown for comparison.
Fig. 9—Load-rotation curves and failure criterion, comparisonfor Tests PG-3 and PG-10 by Guandalini and Muttoni13: (a)analytical and experimental load-rotation curves and failurecriterion according to Eq. (5); (b) geometry of specimens; and(c) geometric and mechanical parameters for each specimen.
Fig. 10—Load-rotation curves and failure criteria for variousreinforcement ratios and slab thicknesses (h = rc =1.2d, rs =rq = 7d, fc = 30 MPa [4200 psi], fy = 500 MPa [71 ksi], anddg = 25 mm [1 in.]).
446 ACI Structural Journal/July-August 2008
For thinner slabs and larger reinforcement ratios, the modeof failure is brittle, generally at values larger than predictedby the ACI equation. For lower reinforcement ratios, but inparticular for thicker slabs, the equations proposed hereinpredict much lower values. This is especially important forthick slabs and foundation mats that may commonly exceeda thickness of 0.4 m (16 in.). In such cases, even for relativelylow reinforcement ratios, the failure mode is brittle andoccurs at load levels clearly below those predicted by ACI,not reaching the theoretical flexural failure load.
Moe’s19 design equation, which remains the basis for thecurrent ACI design equation (Eq. (1)), does not include aterm to account for the effect of the longitudinal reinforcement.It was, however, derived from an analytical expression thatdoes, as explained by Alexander and Hawkins.9 It expressesthe punching shear strength as a function of the ratio VR/Vflex(punching shear strength VR to the load corresponding to thebending capacity Vflex of the slab). Using Eq. (7c), the testseries by Moe19 and Elstner and Hognestad18 can berepresented as in Fig. 11. From the data available at thattime, Moe’s19 conclusion of a linear relationship betweenthe punching shear strength and the ratio VR/Vflex of the slabis confirmed. Shown alongside in the figure as continuouslines are the ultimate loads obtained using the proposedmodel. It can be observed that the level of shear at whichfailure occurs diminishes with increasing thickness of theslab, but the slope remains approximately the same as thatobserved by Moe19 on thin slabs. The size effect is verymarked, especially for thick slabs. For slabs thicker than 0.4 m(16 in.), the ACI 318-056 design equation overestimates thepunching shear strength and does not ensure a ductile behavior.
Also shown in Fig. 11 is the effect of the bending reinforce-ment: increasing this reinforcement increases the punchingshear capacity but simultaneously decreases the ratio of thepunching load to the flexural load, which translates into smaller
rotations at failure. In such cases, the only way to ensure aductile behavior of the slab is to include shear reinforcement.
SIMPLIFIED DESIGN METHODFor practical purposes, the load-rotation relationship can
be further simplified by assuming a parabola with a 3/2exponent for the rotation ψ as a function of the ratio V/Vflexand by assuming that the flexural strength Vflex (refer toEq. (7c)) is reached for a radius of the yielded zone ry equalto 0.75 times the radius of the isolated slab element rs. Theseassumptions, together with Eq. (16), (18), and (22) fromAppendix 1, lead to the following relationship
(8)
Figure 12 shows, again for the four tests by Kinnunen andNylander,8 the experimental load-rotation relationship alongwith those given by Eq. (6) and by the simplified designmethod of Eq. (8). Both expressions correctly predict thepunching load, the simplified design equation giving slightlymore conservative values.
In Table 2, the various expressions proposed in this paper,the complete solution of Eq. (6), and the simplified solutionof Eq. (8) are compared on the basis of nine test series byvarious researchers, for a total of 87 tests. The number oftests in Table 2 is smaller than that of Table 1 because testswith different reinforcement ratios in orthogonal directionsare not considered (tests by Nylander and Sundquist24 andKinnunen et al.25). For tests with square columns, the radiusof the column was assumed to be rc = 2bc/π, where bc is theside of the square column, leading to the same control perimeter.It should be noted that a control perimeter with roundededges is adopted when checking the punching shear strengthaccording to ACI 318-056 (this is the default control perimeteraccording to this code, where it is also permitted a fourstraight-sided control perimeter, refer to Section 11.12.1.3 ofACI 318-056). Similarly, square slabs are transformed intocircular elements with the same flexural strength. Also
ψ 1.5rs
d----
fy
Es
----- VVflex
----------⎝ ⎠⎛ ⎞ 3 2⁄
=
Fig. 11—Punching shear strength as function of V/ Vflexratio for various slab thicknesses and reinforcement ratios(rc = 1.4d, rs = 9.2d, rq = 7.8d, fc = 24 MPa [3400 psi], andfy = 350 MPa [50 ksi]); comparison with tests by Elstnerand Hognestad18 and Moe19 (d =114 mm [4.5 in.], bc =254 mm [10 in.], bs = 1830 mm [72 in.], rq = 890 mm [35 in.],fc = 13 to 51 MPa [1820 to 7180 psi], fy = 303 to 482 MPa[43.1 to 68.6 ksi], and ρ = 0.5 to 7%).
Fig. 12—Plots of load-rotation curves for tests by Kinnunenand Nylander8 (refer to Fig. 8 for geometrical and mechanicalparameters) and comparison to analytical laws of Eq. (6)and (8).
ACI Structural Journal/July-August 2008 447
shown in Table 2 and plotted in Fig. 13 are the results fromACI 318-056 and Eurocode 2.7 The results predicted by theproposed formulations are excellent, with an average ratio ofeffective to predicted load close to unity, and a very smallcoefficient of variation (COV) of 0.08, respectively, 0.09.Also remarkable is the minimum value of the ratio Vtest/Vthgiven in Table 2. A ratio smaller than 1.0 means that theactual strength can be lower than predicted. It is 0.86 for bothproposed formulations.
Tests in which failure occurred after reaching the flexuralstrength of the slab are also included in the results; in thiscase, setting the bending strength to its theoretical value(Eq. (7c)). This is why, in Fig. 13, a series of results areagglutinated along the inclined dotted line that delimits thebending failure mode.
The results given by the simplified Eq. (7) with a bilinearload-rotation relationship, not shown in the table, are verysimilar to those given by the complete solution of Eq. (6).This is not surprising because the considered test seriesinclude, above all, specimens with small or moderate slabthicknesses. By comparisons, the results of ACI 318-056 aregenerally much more conservative, which is to be expectedfrom a design code, but with a much larger COV (0.22 withrounded critical section or 0.20 with a square-sized criticalsection), with the potential to actually lead to unsafe designs(the minimum value of the ratio Vtest/Vth for the consideredtests is 0.82). Furthermore, the ratio Vtest/Vth stronglydecreases for ACI 318-056 with increasing value of theeffective depth of the slab (refer to tests by Hassanzadeh22
and Hallgren10 in Table 2 with d = 200 mm [7.87 in.] or TestPG-3 by Guandalini and Muttoni13 with d = 456 mm [17.9 in.]in Fig. 9).
The results of Eurocode 27 are better, with a smalleraverage of the ratio, and also a smaller COV (average ratioof Vtest/Vth equal to 1.14 and a COV of 0.12 with a minimumvalue of 0.86). It can be noted that Eurocode 27 limits thevalue of the factor affecting size effect for slabs with effectivedepths smaller than 200 mm (7.87 in.) to 2.0 (refer to Eq. (3)),which allows accounting for thickness tolerance for thinslabs. If this limit is not considered, the code equation showsbetter agreement to test results, with an average of 1.02 and
a COV of 0.09, however, the minimum value of the ratioVtest/Vth decreases to 0.79.
Size effectSize effect on punching shear strength was introduced
initially in this paper by multiplying the slab rotation ψ by itsthickness d in the formulation of Eq. (5). It is interesting tonote that a slenderness effect (dependency on the ratio rs/d)is present in the load-rotation relationship given by Eq. (8).Because the rotation according to this equation is inverselyproportional to the slab thickness, if Eq. (8) is introducedinto Eq. (5), the slab thickness d cancels on the right-handside of the equation. Consequently, it follows that the factorfor the reduction of the strength for size effect is not a function
Table 2—Comparison of results of test series with predicted strength of proposed approaches and of current design codes*; average, COV, and minimum value of ratio Vtest /Vth
Reference (year) d, mm (in.) No.
Eq. (5) + Eq. (6) Eq. (5) + Eq. (8) ACI 318-056 EC 27
Average COV Minimum Average COV Minimum Average COV Minimum Average COV Minimum
Elstner and Hognestad18 (1956) 115 (4.52) 22 1.01 0.07 0.88 1.01 0.07 0.86 1.50 0.20 1.05 1.16 0.09 0.95
Kinnunen and Nylander8 (1960) 122 (4.80) 12 1.02 0.09 0.86 1.08 0.08 0.96 1.45 0.18 1.03 1.14 0.13 0.90
Moe19 (1961) 114 (4.48) 9 1.06 0.09 0.94 1.07 0.09 0.98 1.51 0.10 1.25 1.22 0.07 1.13
Schäfers20 (1984)113 to 170
(4.45 to 6.69) 4 1.02 0.08 0.93 1.06 0.10 0.94 1.41 0.14 1.16 1.25 0.05 1.19
Tolf21 (1988)98 to 200
(3.86 to 7.87) 8 0.98 0.10 0.87 1.06 0.10 0.92 1.33 0.21 0.98 1.11 0.14 0.94
Hassanzadeh22 (1996) 200 (7.87) 3 0.97 0.09 0.87 1.04 0.08 0.95 1.10 0.06 1.03 1.03 0.14 0.86
Hallgren10 (1996) 199 (7.83) 7 0.94 0.04 0.90 1.06 0.07 0.96 1.05 0.09 0.90 0.96 0.05 0.90
Ramdane24 (1996) 98 (3.86) 12 1.07 0.08 0.94 1.16 0.08 1.03 1.43 0.23 0.91 1.22 0.12 1.00
Guandalini and Muttoni13 (2004)96 to 464
(3.78 to 18.2) 10 1.07 0.08 0.95 1.14 0.08 1.02 1.16 0.24 0.82 1.04 0.09 0.90
Σ 87 1.02 0.08 0.86 1.07 0.09 0.86 1.37 0.22 0.82 1.14 0.12 0.86*Tests with different bending reinforcement ratios along orthogonal directions not included.Note: COV = coefficient of variation.
Fig. 13—Comparison of various formulations of ACI 318-05,6
Eurocode 2,7 and combination of Eq. (5) and (6) and of Eq. (5)and (8) with test results shown in Fig. 5 and Table 2.
448 ACI Structural Journal/July-August 2008
of the slab thickness, but rather of the span, represented inEq. (8) by the radius rs of the isolated slab element.
CODE-LIKE FORMULATIONIn 2003, Muttoni17 proposed a similar relationship for the
failure criterion for punching shear of flat slab systemsassuming that rs = 0.22L, where L is the span of the slab, andthat the flexural capacity of the slab is Vflex ≅ 8mRd (wheremRd is the flexural capacity of the slab in the column regionreduced by the strength reduction factor). The resulting load-rotation relationship is thus
(9)
where Vd is the factored shear force. Here again, the rotation isslenderness-dependent and thus it is inversely proportionalto the thickness of the slab, with the consequence that thesize effect factor of Eq. (5) is again a function of the span Lof the slab and not of its thickness. Equation (9) is formulatedfor intermediate columns; for edge columns, the constant 8is to be replaced by 4 and for corner columns by 2.
Equation (5), in a slightly rearranged form and to reach atarget fractile of 5%, including a model factor to cover someirregularities in the spans and in disposition of the loading,has been introduced in the Swiss Code for structural concreteSIA 26227 as
(10)
where γc is the partial safety factor of concrete (γc = 1.5) or
where φ is the strength reduction factor for punching (φ = 0.75).
Design approachIt is possible to combine Eq. (9) describing the load-
deflection behavior of the slab element with the failurecriterion of Eq. (10) into a single design formula. The exact
ψ 0.33Ld---
fy
Es
-----Vd
8mRd
------------⎝ ⎠⎛ ⎞ 3 2⁄
=
VRd
b0d fc′------------------ 2
3γc
------- 1
1 20 ψddg0 dg+-------------------+
----------------------------------- (SI units: N, mm)=
VRd
b0d fc′------------------- φ
8
1 20 ψddg0 dg+--------------------+
------------------------------------ (U.S. customary units: psi, in.)=
punching strength (Point A in Fig. 14) is then obtained bysetting VRd equal to Vd and iteratively solving the resultingequation. Requiring an iterative calculation even for thesimplest cases, this formulation would not be very useful inpractice. Instead, a simple design check can be performedcalculating the slab rotation ψd corresponding to the factoredshear force Vd using Eq. (9). From that value, the correspondingpunching shear strength of the slab (Point B of Fig. 14) isfound by applying Eq. (10). If the strength obtained fromEq. (10) is larger than the design load Vd, the design is safeand conservative. If, on the contrary, it is insufficient, theflexural reinforcement, the column size, or the slab thicknesshas to be increased.
Parametric study and comparison to test resultsFigure 15 demonstrates the ability of the proposed
formulation to investigate various aspects of the phenomenonof punching shear. As already known, an increase in thebending reinforcement leads to an increase in the punchingshear capacity (Fig. 15(a)). This effect is not considered inthe ACI 318-056 formulation, but is included in Eurocode 27
and the proposed formulation (where an increase in thebending reinforcement reduces the slab rotation ψ).
The effect of the size of the column relative to the thicknessof the slab is illustrated in Fig. 15(b). This effect is consideredby ACI, but only for large values of the ratio b0/d. Theproposed formulation, again, correctly describes this effectfor the available test results, as does the formulation ofEurocode 2,7 which handles it by working with a controlperimeter located at 2d from the column face instead of d/2for ACI and the present paper.
Figure 15(c) shows the effect of the effective slab thicknesson the punching strength. The few available tests pointtoward a strong decrease for very thick slabs, which iscorrectly described by the proposed model and Eurocode 27
but ignored by ACI.Concerning the effect of concrete strength on punching
shear, Eurocode 27 and the proposed formulation giveconsistently good results, as shown in Fig. 15(d).
The effect of the type of steel used and of its yield stress fyhas been the object of only limited investigations, mostly byMoe.19 This effect is not very pronounced, but a slightincrease with increasing yield stress is predicted by theproposed formulation.
The span-depth ratio of the slab, represented by the ratiors/d for isolated slab elements also has an effect on thepunching shear strength, according to the proposed formulation.This effect is considered neither by ACI 318-056 nor byEurocode 2.7 Further research should be devoted to investigatethis aspect, as the punching strength of very slender slabsappears to be lower than expected, and no tests with significantthickness are currently available.
SUMMARY AND CONCLUSIONSDesign rules for punching shear present in design codes
are generally based on experimental results performed onisolated slab elements representing the part of the slab closeto the column. Most tests have been performed on relativelythin slabs, typically 0.1 to 0.2 m (4 to 8 in.). The test resultsare nonetheless commonly extrapolated to design flat slabswith a thickness typically 2 to 3 times larger, and even forfoundation mats with thicknesses 10 to 20 times larger.
The present paper proposes a mechanical model based onthe critical shear crack theory, explaining punching behaviorFig. 14—Design procedure to check punching strength of slab.
449ACI Structural Journal/July-August 2008
of flat slabs without shear reinforcement and correctlyaccounting for size effect. A failure criterion is derived on itsbasis, which suitably describes the role of the manygeometric and mechanical parameters involved in punchingshear. The main conclusions of this paper are:
1. According to the proposed failure criterion, the punchingstrength is a function of the opening of a critical shear crackin the slab. Its influence is assumed to be proportional to theproduct of the slab rotation times the slab thickness andcorrected by a factor to account for the maximum diameterof the aggregate;
2. This failure criterion simultaneously determines thepunching load and the rotation capacity of the slab, and thusof its ductility;
3. The punching load can be determined by applying thefailure criterion and a load-rotation relationship obtainedfrom a nonlinear analysis of the slab in bending. For axisym-metric cases, an analytical formulation derived on the basisof a nonlinear moment-curvature diagram is given;
4. A simplified bilinear (elasto-plastic) moment-curvaturerelationship can also be applied to accurately estimate thepunching load. The use of a more sophisticated moment-curvature relationship is only required for thick slabs withlow reinforcement ratios, in which it is necessary to precisely
account for the effects of the tensile strength of concrete andof tension stiffening;
5. A simplified analytical formulation of the load-rotationrelationship, as it is used in the current Swiss design codefor concrete structures, also gives a good estimate of thepunching load;
6. The article proposes a method to calculate the punchingstrength as a function of the effective depth of the slab, the sizeof the column, the flexural reinforcement ratio, the yieldstrength of the reinforcing steel, the concrete strength, themaximum aggregate size, and the span-depth ratio of the slab.This method gives very good results when compared with aseries of 87 test results, with a COV of the ratio Vtest/Vth of 8%;
7. Size effect on the punching shear strength is accountedin the failure criterion of the critical shear crack theory. Thiseffect, in combination with the slenderness effect on theload-rotation relationship proposed in this paper, can beformulated as a function of the span of the slab;
8. ACI 318-056 does not only exhibit a very large COV whencompared with test results (22%), but it does not includeimportant effects, which leads to unsafe designs in particularfor thick and/or slender slabs with low reinforcement ratios;
Fig. 15—Comparison of punching shear strength according to ACI 318-05,6 Eurocode 2,7 and the refined (Eq. (5) and (6)) andsimplified (Eq. (5) and (8)) methods proposed in this paper with various test results showing influence of: (a) reinforcement ratio(tests by Elstner and Hognestad18); (b) punching shear perimeter (tests by Hassanzadeh22 and Tolf21); (c) effective depth ofslab (tests by Guandalini and Muttoni13); (d) concrete strength (tests by Ramdane23); (e) yield strength of steel (tests byMoe19); and (f) slenderness of slab.
450 ACI Structural Journal/July-August 2008
9. Eurocode 27 has a better COV when compared with testresults (12%), but it also can predict unconservative valuesfor slender slabs;
10. Even if tests on thin slabs have exhibited some level ofductility for low reinforcement ratios, the behavior is quitebrittle for thicker slabs; and
11. For thick slabs, the only solution to reach a satisfactorylevel of ductility is to place punching shear reinforcement.
ACKNOWLEDGMENTSThe work presented in this paper was funded by the Association of the
Swiss Cement Industry (cemsuisse) and by the Swisscode project of theSwiss Society of Engineers and Architects (SIA). The author is appreciativeof the support received.
REFERENCES1. Gasparini, D. A., “Contributions of C. A. P. Turner to Development of
Reinforced Concrete Flat Slabs 1905-1909,” Journal of StructuralEngineering, ASCE, V. 128, No. 10, 2002, pp. 1243-1252.
2. Fürst, A., and Marti, P., “Robert Maillart’s Design Approach for FlatSlabs,” Journal of Structural Engineering, ASCE, V. 123, No. 8, 1997,pp. 1102-1110.
3. Silfwerbrand, J., and Hassanzadeh, G., eds., “International Workshopon Punching Shear Capacity of RC Slabs,” Royal Institute of Technology,Stockholm, Sweden, 2000, 527 pp.
4. FIB, “Punching of Structural Concrete Slabs,” fib Bulletin 12,Lausanne, Switzerland, 2001, 307 pp.
5. Polak, M. A., ed., Punching Shear in Reinforced Concrete Slabs, SP-232,American Concrete Institute, Farmington Hills, MI, 2005, 302 pp.
6. ACI Committee 318, “Building Code Requirements for StructuralConcrete (ACI 318-05) and Commentary (318R-05),” American ConcreteInstitute, Farmington Hills, MI, 2005, 430 pp.
7. Eurocode 2, “Design of Concrete Structures—Part 1-1: General Rulesand Rules for Buildings,” CEN, EN 1992-1-1, Brussels, Belgium, 2004,225 pp.
8. Kinnunen, S., and Nylander, H., “Punching of Concrete Slabs WithoutShear Reinforcement,” Transactions of the Royal Institute of Technology,No. 158, Stockholm, Sweden, 1960, 112 pp.
9. Alexander, S. D. B., and Hawkins, N. M., A Design Perspective onPunching Shear, SP-232, M. A. Polak, ed., American Concrete Institute,Farmington Hills, MI, 2005, pp. 97-108.
10. Hallgren, M., “Punching Shear Capacity of Reinforced HighStrength Concrete Slabs,” doctoral thesis, Royal Institute of Technology,Stockholm, Sweden, 1996, 206 pp.
11. Broms, C. E., Concrete Flat Slabs and Footings: Design Method forPunching and Detailing for Ductility, Royal Institute of Technology,Stockholm, Sweden, 2006, 114 pp.
12. Muttoni, A., and Schwartz, J., “Behaviour of Beams and Punching inSlabs without Shear Reinforcement,” IABSE Colloquium, V. 62, Zurich,Switzerland, 1991, pp. 703-708.
13. Guandalini, S., and Muttoni, A., “Symmetric Punching Tests onReinforced Concrete Slabs without Shear Reinforcement,” Test report,EPFL, Lausanne, Switzerland, 2004, 78 pp. (in French)
14. Bollinger, K., “Load-Carrying Behaviour and Reinforcement ofAxisymmetrically Loaded Reinforced Concrete Plates,” doctoral thesis,Abteilung Bauwesen der Universität Dortmund, Dortmund, Germany,1985, 262 pp. (in German)
15. Walraven, J. C., “Fundamental Analysis of Aggregate Interlock,”Journal of Structural Engineering, ASCE, V. 107, No. 11, 1981, pp. 2245-2270.
16. Vecchio, F. J., and Collins, M. P., “The Modified Compression-FieldTheory for Reinforced Concrete Elements Subjected to Shear,” ACIJOURNAL, Proceedings V. 83, No. 2, Mar.-Apr. 1986, pp. 219-231.
17. Muttoni, A., “Shear and Punching Strength of Slabs without ShearReinforcement,” Beton-und Stahlbetonbau, V. 98, No. 2, Berlin, Germany,2003, pp. 74-84. (in German)
18. Elstner, R. C., and Hognestad, E., “Shearing Strength of ReinforcedConcrete Slabs,” ACI JOURNAL, Proceedings V. 53, No. 2, Feb. 1956,pp. 29-58.
19. Moe, J., “Shearing Strength of Reinforced Concrete Slabs and Footingsunder Concentrated Loads,” V. D47, PCA, IL, 1961, 135 pp.
20. Schäfers, U., “Construction, Dimensioning and Safety with Respectto Punching Shear of Reinforced Concrete Flat Plates in the Vicinity ofInternal Columns,” Deutscher Ausschuss für Stahlbeton, No. 357, Berlin,Germany, 1984, 83 pp. (in German)
21. Tolf, P., “Influence of the Slab Thickness on the Strength of ConcreteSlabs at Punching: Tests with Circular Slabs,” No. 146, Royal Institute ofTechnology, Stockholm, Sweden, 1988, 64 pp. (in Swedish)
22. Hassanzadeh, G., “Strengthening of Bridge Slabs with Respect toPunching: Test Results,” Report 41, Royal Institute of Technology, Stockholm,Sweden, 1996, 134 pp. (in Swedish)
23. Ramdane, K.-E., “Punching Shear of High Performance ConcreteSlabs,” Utilization of High-Strength/High Performance Concrete,Proceedings of the Fourth International Symposium, V. 3, Paris, France,1996, pp. 1015-1026.
24. Nylander, H., and Sundquist, H., “Punching of Bridge Slabs withNon-Prestressed Reinforcement on Columns,” No. 104, Royal Institute ofTechnology, Stockholm, Sweden, 1972, 64 pp. (in Swedish)
25. Kinnunen, S.; Nylander, H.; and Tolf, P., “Influence of the SlabThickness on the Strength of Concrete Slabs at Punching: Tests withRectangular Slabs,” Test Report, Royal Institute of Technology, No. 137,Stockholm, Sweden, 1980, 73 pp. (in Swedish)
26. Guandalini, S., “Symmetric Punching in R/C Slabs,” doctoral thesis,No. 3380, EPFL, Lausanne, Switzerland, 2005, 289 pp. (in French)
27. SIA, “262 Code for Concrete Structures,” Swiss Society of Engineersand Architects, Zurich, Switzerland, 2003, 94 pp.
18
APPENDIX 1 1
In this appendix, a load-rotation relationship for an isolated slab element is derived based on the 2
assumption that the deflected shape of the isolated slab element is conical outside the critical shear 3
crack. The curvature in tangential direction (Fig. 6f) is thus: 4
rt
ψχ −= for r > r0 (11) 5
Inside the critical shear crack, it may be assumed that the curvatures in both directions are constant 6
and equal (Figs 6d,f), so that the deflected shape is spherical : 7
0rtr
ψχχ −== for r < r0 (12) 8
With these curvatures, the internal forces described in Figs 6b,c can be calculated according to the 9
quadrilinear moment-curvature relationship shown in Fig. 7. This relationship is characterized by 10
the stiffnesses EI0 before and EI1 after cracking, the cracking moment mcr , the moment capacity mR 11
and the tension stiffening effect χTS. Neglecting the effect of reinforcement before cracking, these 12
terms can be obtained as: 13
6
2hfm ctcr
⋅= (13) 14
12
3
0hE
EI c ⋅= (14) 15
c
ctcrcr Eh
fEIm
⋅⋅
==−2
0
χ (15) 16
Assuming a linear-elastic behaviour of steel and concrete after cracking, it follows: 17
⎟⎠⎞
⎜⎝⎛ −⋅⎟
⎠⎞
⎜⎝⎛ −⋅⋅⋅⋅=
dc
dcdEEI s 3
1131 βρ (16) 18
where c is the depth of the compression zone: 19
⎟⎟⎠
⎞⎜⎜⎝
⎛−
⋅⋅⋅
+⋅⋅⋅⋅= 12
1s
c
c
s
EE
dEE
cβρ
βρ (17) 20
19
and β is an efficiency factor that accounts for the orthogonal layout of the reinforcement and the 1
reduction in the ratio between the torsion and bending stiffness of the slab after cracking. It should 2
be noted that this factor affects the stiffness of the member but not the flexural strength of the 3
member. While the developments above were made for a layout with a polar symmetry 4
(reinforcement placed in radial and tangential directions), reinforcement is usually placed 5
orthogonally in the slab. For these cases, a good agreement to test data is obtained assuming 6
β = 0.6. 7
Assuming a perfectly plastic behaviour of the reinforcement after yielding, a rectangular stress 8
block for concrete in the compression zone and neglecting compression reinforcement, the moment 9
capacity mR of the section is then: 10
⎟⎟⎠
⎞⎜⎜⎝
⎛⋅
⋅−⋅⋅⋅=
c
yyR f
fdfm
212 ρ
ρ (18) 11
The decrease in curvature caused by tension stiffening can be approximated by the constant 12
contribution χTS : 13
hEf
s
ctTS ⋅
⋅⋅⋅
=6
1βρ
χ (19) 14
which corresponds approximately to 0.5 · mcr / EI1. 15
The curvatures χ1 at the beginning of the stabilized cracked regime and χy at yielding are thus: 16
TScr
EIm
χχ −=−1
1 (20) 17
and 18
TSR
y EIm
χχ −=−1
(21) 19
The four segments of the assumed moment-curvature relationship correspond to the four regions of 20
the slab shown in Figs 6f,g. The radii delimiting these zones may be determined by substituting 21
Eqs (15), (20) and (21) into Eq. (11), as follows: 22
Zone within which the reinforcement is yielding, plastic radius ry : 23
20
s
TSRy
y r
EIm
r ≤−
=−=χ
ψχψ
1
(22) 1
Zone in which cracking is stabilized, radius r1: 2
s
TScr
r
EImr ≤
−=−=
χ
ψχψ
1
11 (23) 3
and zone up to which the concrete is cracked, cracking radius rcr : 4
scrcr
cr rm
EIr ≤
⋅=−= 0ψ
χψ (24) 5
The equilibrium equation of the slab portion shown in Fig. 6c is: 6
( ) drmrmrrVsr
rrcq ⋅⋅∆−⋅∆⋅−=−⋅
∆⋅ ∫
0
0π2 ϕϕϕϕ (25) 7
where mr is the radial moment at r = r0 calculated according to Fig. 7 with the curvature given by 8
Eq. (12). It follows that: 9
⎟⎟
⎠
⎞
⎜⎜
⎝
⎛
−⋅⋅+−⋅+−⋅⋅
+−⋅⋅+−⋅+⋅−⋅
−=
)ln()ln(
)ln()ln(π2
0111
1100
crscrcryTS
yyRr
cq rrEIrrmrrEI
rrEIrrmrm
rrV
ψχ
ψ (6) 10
where the operator x is x for 0≥x and 0 for 0<x 11
12
APPENDIX 2 13
The following symbols are used in the paper: 14
Ec = modulus of elasticity of concrete (assumed 31
000'10 cc fE ⋅= [MPa], 15
31
000'276 cc fE ⋅= [psi]) 16
Es = modulus of elasticity of reinforcement 17
EI0 = flexural stiffness before cracking 18
EI1 = tangential flexural stiffness after cracking 19
L = main span of a slab system 20
21
V = shear force 1
Vd = factored shear force 2
Vflex = shear force associated with flexural capacity of the slab 3
VR = nominal punching shear strength 4
VRd = design punching shear strength 5
Vtest = experimental punching shear strength 6
Vth = theoretical punching shear strength 7
b0 = perimeter of the critical section for punching shear 8
bc = side length of a square column 9
bs = side length of a square isolated slab element 10
c = distance from extreme compression fibre to neutral axis 11
d = distance from extreme compression fibre to the centroid of the longitudinal 12
tensile reinforcement 13
db = diameter of a reinforcement bar 14
dg = maximum diameter of the aggregate 15
dg0 = reference aggregate size (16 mm (0.63 in)) 16
fc = average compressive strength of concrete (cylinder) 17
f 'c = specified compressive strength of concrete (cylinder) 18
fct = tensile strength of concrete (assumed 32
3.0 cct ff ⋅= [MPa], 32
6.1 cct ff ⋅= [psi]) 19
fy = yield strength of reinforcement 20
h = slab thickness 21
mcr = cracking moment per unit width 22
mr = radial moment per unit width 23
mt = tangential moment per unit width 24
mR = nominal moment capacity per unit width 25
mRd = design moment capacity per unit width 26
22
r = radius 1
r0 = radius of the critical shear crack 2
r1 = radius of the zone in which cracking is stabilized 3
rc = radius of a circular column 4
rcr = radius of cracked zone 5
rq = radius of the load introduction at the perimeter 6
rs = radius of circular isolated slab element 7
ry = radius of yielded zone 8
∆ϕ = angle of a slab sector 9
β = efficiency factor of the bending reinforcement for stiffness calculation 10
γ c = partial safety factor for concrete (according to European practice, γ c = 1.5) 11
ρ = reinforcement ratio 12
φ = strength reduction factor (according to North-American practice, φ = 0.75 for shear) 13
χ1 = curvature in stabilized cracking 14
χcr = curvature at cracking 15
χr = curvature in radial direction 16
χt = curvature in tangential direction 17
χy = yielding curvature 18
χTS = decrease in curvature due to tension stiffening 19
ψ = rotation of slab outside the column region 20
ψd = rotation of slab outside the column region due to factored shear force Vd 21
ξ = size effect coefficient in Eurocode 27 22